Abstract
The topological materials have attracted much attention for their unique electronic structure and peculiar physical properties. ZrTe_{5} has host a longstanding puzzle on its anomalous transport properties manifested by its unusual resistivity peak and the reversal of the charge carrier type. It is also predicted that singlelayer ZrTe_{5} is a twodimensional topological insulator and there is possibly a topological phase transition in bulk ZrTe_{5}. Here we report highresolution laserbased angleresolved photoemission measurements on the electronic structure and its detailed temperature evolution of ZrTe_{5}. Our results provide direct electronic evidence on the temperatureinduced Lifshitz transition, which gives a natural understanding on underlying origin of the resistivity anomaly in ZrTe_{5}. In addition, we observe onedimensionallike electronic features from the edges of the cracked ZrTe_{5} samples. Our observations indicate that ZrTe_{5} is a weak topological insulator and it exhibits a tendency to become a strong topological insulator when the layer distance is reduced.
Introduction
The transition metal pentatellurides like ZrTe_{5} and HfTe_{5} (ref. 1) have attracted considerable interest since the last 70s because they exhibit unusual transport properties characterized by a strong resistivity peak^{2,3} accompanied by a sign reversal of the Hall coefficient and thermopower across the peak temperature^{4,5,6}. The origin of such transport property anomalies has been a subject of a longtime debate but remains unclear, with explored possibilities of structural phase transition^{3,7}, formation of a charge/spin density wave^{8}, polaronic behaviour^{9}, a semimetal–semiconductor transition^{6} or temperatureinduced band shift^{10}. With the emergence of topological materials, including topological insulators^{11,12,13}, threedimensional Dirac semimetals^{14,15,16,17,18,19,20,21,22,23} and threedimensional Weyl semimetals^{24,25,26,27,28,29,30,31,32,33}, ZrTe_{5} and HfTe_{5} have ignited renewed interest as a candidate of a novel topological material. While many threedimensional topological insulators have been predicted and discovered, twodimensional topological insulators, also known as quantum spin Hall insulators that can support topologically protected helical edge modes inside a bulk insulating gap and lead to dissipationless transport, are rare^{34,35,36}, especially in natural compounds^{13}. It was predicted that singlelayer ZrTe_{5} is a twodimensional topological insulator with a large bulk bandgap, while bulk ZrTe_{5} may host a possibility of realizing a temperaturedriven topological phase transition between the weak and strong topological insulators^{37}. However, a number of recent experiments on ZrTe_{5} point to its being a threedimensional Dirac semimetal^{38,39,40} or a quasitwodimensional Dirac semimetal^{41}. Added to the interest of ZrTe_{5} is the recent observation of superconductivity under high pressure^{42}. Direct investigation on the electronic structure of ZrTe_{5} is highly desired in understanding the electronic origin of the transport property anomaly, and in uncovering the exact nature of the topological state in ZrTe_{5}. Angleresolved photoemission spectroscopy (ARPES)^{43} can provide direct information on the electronic structure of materials in addressing the abovementioned prominent issues in ZrTe_{5}. However, highresolution comprehensive ARPES measurements on ZrTe_{5}, especially the lowenergy electronic structure, are still lacking^{6,10,38}.
In this paper, we present detailed ARPES measurements on ZrTe_{5} with unprecedented energy and momentum resolutions, by taking advantage of our latestgeneration laserbased ARPES system, which can cover twodimensional momentum space simultaneously. For the first time, we find that the electronic property of ZrTe_{5} is dominated by two branches of bands with nearly linear dispersion, a valence band and a conduction band, at the Brillouin zone centre. There is an energy gap that separates these two branches of bands; the gap decreases with decreasing temperature but persists to a very low temperature (∼2 K). The overall electronic structure exhibits a marked temperature dependence that shifts down with decreasing temperature. This results in an evolution from a ptype semimetal with a holelike Fermi pocket at high temperature above 135 K, to a semiconductor around 135 K where its resistivity shows a peak, to an ntype semimetal with an electronlike Fermi pocket at low temperature. These results constitute direct electronic evidence of a temperatureinduced Lifshitz transition in ZrTe_{5}. They provide a natural understanding on the underlying origin of the resistivity anomaly at ∼135 K and its sign reversal of Hall coefficient and thermopower across the same temperature. We also observe onedimensionallike electronic features associated with the edges of some cracked ZrTe_{5} samples. Our observations indicate that ZrTe_{5} is a weak topological insulator that shows a tendency to become a strong topological insulator when the layer distance is reduced.
Results
Sample characterization
ZrTe_{5} is a layered compound that crystallizes in the orthorhombic crystal structure^{1}. It is constructed from layerstacking of the ZrTe_{5} sheets along the b axis. The twodimensional ZrTe_{5} sheet (Fig. 1a) features a trigonal prismatic ZrTe_{6} chains running along the a axis that are linked together along the c axis via zigzag chains of Te atoms. Each ZrTe_{5} sheet is nominally charge neutral, and the distance between the adjacent two ZrTe_{5} sheets along the b axis is quite large (∼7.25 Å), giving rise to a weak interlayer coupling^{37}. Figure 1b shows the projected surface Brillouin zone for ZrTe_{5} with the high symmetry momentum points labelled in a standard way. Figure 1c shows the morphology of a cleaved ZrTe_{5} surface that is smooth and mirrorlike; the data presented in Figs 1, 2, 3 were taken on this kind of surface. The resistivitytemperature data of our ZrTe_{5} sample (Fig. 1d) exhibits a prominent peak at ∼135 K. This is consistent with the typical ZrTe_{5} samples reported before^{2,3,4,6,7,8,9,10,41,42,44,45} (see Methods for the sample details).
Fermi surface and band structure
The ARPES data are taken with our new laserbased system equipped with the latestgeneration timeofflight analyser. It not only has high energy and momentum resolutions but also has a new capability of covering twodimensional momentum space simultaneously (see Methods for experimental details). Figure 1e–h shows the constant energy contours of ZrTe_{5} measured at 195 K, which represent the spectral intensity distribution at the Fermi level (Fig. 1e) and at a few binding energies of 100 (Fig. 1f), 200 (Fig. 1g) and 300 meV (Fig. 1h). The corresponding band structures are shown in Fig. 1i–l measured along several typical momentum cuts as indicated in Fig. 1h. We have checked the effect of the polarization geometry on the measured results. The measured constant energy contours and band structures are similar under two typical s and p polarization geometries, although the spectral weight distribution in the momentum space shows a clear polarization dependence (Supplementary Fig. 1).
The constant energy contour at the Fermi level shows a tiny spot at the Brillouin zone centre, Γ point (Fig. 1e). With increasing binding energy, it grows in area and evolves into a warped rectangle at high binding energies of 200 (Fig. 1g) and 300 meV (Fig. 1h). This is consistent with the observation of holelike bands below the Fermi level as seen in Fig. 1i–l. These holelike bands show nearly linear dispersions over a wide energy range. They also exhibit a strong anisotropy: the bands are steeper along the horizontal or vertical highsymmetry directions (Fig. 1i,k for cuts 1 and 3 in Fig. 1h) with a Fermi velocity of ∼4 eV·Å (corresponding to 6.3 × 10^{5} m s^{−1}, 1/480 c with c being the speed of light) than those along the momentum cuts 2 (Fig. 1j) and 4 (Fig. 1l) with a Fermi velocity of ∼2.3 eV·Å (corresponding to 3.6 × 10^{5} m s^{−1}, 1/830 c). Detailed lineshape analysis of these holelike bands at Γ indicates that they are broad; the corresponding photoemission spectra (energy distribution curves, EDCs) are not composed of a single sharp peak or two sharp peaks, but represent a spectral continuum encompassed by two edges (Supplementary Fig. 2).
To understand the measured electronic structure, we have performed band structure calculations of ZrTe_{5} (see Methods for details of the band structure calculations). The calculated band structures (Supplementary Figs 3 and 4) and constant energy contours (Supplementary Fig. 5) are basically consistent with the previous reports^{37,46}. The evolution of the constant energy contours near Γ point with the increasing binding energy (Fig. 1e–h) from a spot to a small circle to a warped rectangle is in good agreement with the calculated results (Supplementary Fig. 5), considering a chemical potential difference in the comparison. Band structure calculations on bulk ZrTe_{5} give only one sharp holelike band near Γ in this case that is apparently not consistent with our measurements. The slab calculations (Supplementary Fig. 4b), on the other hand, provide a good explanation on this behaviour. This broad band feature can be understood reasonably well by the finite k_{z} effect, consistent with the results of the slab band calculations (Supplementary Fig. 4b,d).
Temperature evolution of the electronic structures
We have carried out detailed ARPES measurements on ZrTe_{5} at different temperatures to understand the origin of the anomalous transport properties and examine on possible temperatureinduced topological phase transition. Figure 2 shows the temperature dependence of the energy bands measured along two highsymmetry momentum cuts. The corresponding temperature dependence of the constant energy contours is shown in Fig. 3. These results are highly reproducible by measuring on the same sample with cycles of cooling down and warming up (Supplementary Fig. 6), by cleaving samples at high and low temperatures, and by measuring on many different samples. The band images (Fig. 2a,b) are obtained by dividing the original data with their corresponding Fermi distribution functions, making it possible to reveal features above the Fermi level at relatively high temperatures.
From Fig. 2a,b, it is clear that the band structure near Γ consists of two branches, one is the upper branch (UB) at lower binding energy or above the Fermi level that corresponds to the electronlike conduction band, while the other is the lower branch (LB) at high binding energy that corresponds to the holelike valence band. In between the UB and LB bands, there is a region with strongly suppressed spectral weight that we call it valley region. The bands at Γ point show a strong temperature dependence; the overall band structure shifts down to high binding energy with decreasing temperature. Specifically, the LB band touches the Fermi level at high temperature (255 K in Fig. 2a,b); it shifts down with decreasing temperature and sinks well below the Fermi level at low temperatures. On the other hand, the UB band is well above the Fermi level at high temperature (255 K in Fig. 2a,b), moves down with decreasing temperature and crosses the Fermi level at very low temperature (for example, 35 and 2 K in Fig. 2a,b). Such a band shift with temperature is consistent with those reported before^{6,10}.
Although the overall band structure shifts down with decreasing temperature, we find that it is not a rigid band shift. To keep track on the temperature evolution of the bands in a more quantitative way, we plot the photoemission spectra (EDCs) at Γ point measured at different temperatures in Fig. 2c. The EDCs consist of signals from the LB band and the UB band, with a valley separating in between them. The LB band is visible in the entire measured temperature range, which is encompassed by a lowerbindingenergy upper edge and highbindingenergy lower edge. The UB band is invisible above E_{F} at high temperatures (255 K), moves down with decreasing temperature and part of it becomes visible at low temperatures. Figure 2d shows the energy positions of the upper edge of the LB band, lower edge of the LB band and the centre of the valley bottom. The two edges of the LB band and the valley centre show a similar trend of temperature dependence; the overall energy shift from 255 to 2 K is on the order of ∼70 meV. A close examination indicates that the LB band gets wider with decreasing temperature as seen from the energy difference between the upper and lower edges of the LB band (Fig. 2e). On the other hand, the Ushaped valley becomes steeper with decreasing temperature, seen from the energy difference between the upper edge of the LB band and the valley centre (Fig. 2e). These indicate that the band shift with temperature is not a strictly rigid band shift. We notice that 135 K is a characteristic temperature where the valley centre crosses the Fermi level (Fig. 2c,d). We also note that the energy shift of bands near Γ with temperature is faster in the hightemperature region of 165–255 K than that in the lowertemperature 2–105 K region (Fig. 2d).
The strong suppression of the spectral weight in the valley region is indicative of an gap opening between the LB band and the UB band (Fig. 2a,b). As seen in Fig. 2c, at high temperatures, the valley bottom in EDCs shows a flat region with an intensity close to zero when taking the signal background into account. This suggests a true gap opening at high temperatures. We estimate the gap size in two ways. In the first method, we choose the highbindingenergy region at 0.30–0.35 eV in EDCs, which is very weak and slightly above zero intensity as the background line. The line intersects with the valley bottom at two points and the distance between these two points are taken as an estimation of the gap size. Compared with zero intensity background, this method slightly overestimates the gap size, but it provides an objective and direct way in extracting the gap value and the difference is small compared to that obtained from zero intensity background. The energy gap obtained in this way is large at high temperatures (∼40 meV for 255 K), and gets smaller with decreasing temperature (Fig. 2f). At very low temperatures, such as 35 and 2 K, the spectral weight near the valley bottom increases that is above the zero intensity. In this case, there is no more true gap opening so we cannot determine the gap size using the same criterion as used at high temperatures. However, we believe there remains a gap opening near the valley region because the spectral weight is still strongly suppressed, a situation similar to the pseudogap observed in hightemperature cuprate superconductors^{43}. It is also possible that besides a true gap opening there is a new ingap state produced by other mechanism that fills in the gap region and grows with decreasing temperature. If there is no gap opening and a Dirac conelike structure is formed, one would expect to see a peak at the Dirac point that is not consistent with the present result. This leads us to take another way to estimate the gap size. If we assume a Dirac cone structure as a reference point that has zero gap, the gap opening would split the LB and the UB bands, and causes a spectral weight suppression at the gapped valley region. In this case, the distance between the LB and the UB bands can be used as a measure of the gap size. Assuming the LB and the UB bands show similar temperaturedependent splitting from the valley centre, the gap size can be estimated as twice the distance between the position of the upper edge of the LB band and the position of the valley centre, as shown in Fig. 2f (red empty circles). In this case, the gap size still decreases with decreasing temperature, but it persists in the entire temperature range we have measured.
Temperatureinduced Lifshitz transition
The temperature dependence of the Fermi surface provides a clear evidence of a temperatureinduced Lifshitz transition in ZrTe_{5}. Figure 3 shows the temperature evolution of the constant energy contours at the Fermi level (Fig. 3a) and at a binding energy of 100 meV (Fig. 3b) for ZrTe_{5}. The corresponding momentum distribution curves across the Γ point at different temperatures are shown in Fig. 3c–f for the two cases, which provide information on the temperature evolution of the pocket size (Fig. 3g) and the spectral weight at the Fermi level (Fig. 3h). At a high temperature like 255 K, there is a tiny holelike pocket at Γ (leftmost panel in Fig. 3a), consistent with a holelike band crossing the Fermi level in Fig. 2a,b. With decreasing temperature, the pocket near Γ shrinks in size, becomes invisible at 135 K, then emerges again below 135 K. Its size increases with further decreasing of temperature and it becomes an electronlike pocket as seen from bands in Fig. 2a,b. Therefore, there is a clear Lifshitz transition that occurs across ∼135 K where the Fermi surface topology transforms from a holelike pocket at high temperature to an electronlike pocket at low temperature. It is interesting to note that a temperatureinduced Lifshitz transition is also reported in another transition metal dichalcogenide WTe_{2} (ref. 47). For the constant energy contours at a binding energy of 100 meV (Fig. 3b), the pocket size at the Γ point keeps shrinking with decreasing temperature, as seen from the distance of two peaks in momentum distribution curves (Fig. 3e,f,i). As seen in Fig. 2, the band at 100 meV binding energy represents solely the LB valence band over the entire temperature range we measured. It is natural that the pocket size shrinks when the holelike band moves to high binding energy with decreasing temperature. In addition to the bands at Γ point, we also observe another band (denoted as β band) that crosses the Fermi level at low temperature and forms four electron pockets at Brillouin zone boundary when we scan the entire momentum space of the first Brillouin zone (Supplementary Fig. 7). This is consistent with the band structure calculations (Supplementary Fig. 5d). Together with the Γ point bands, the β band also shifts down when temperature decreases (Supplementary Fig. 8). Except for the near Γ point bands and β band described above, no other band is detected over the entire first Brillioun zone in the temperature range we measured (Supplementary Fig. 7).
Discussion
The identification of a temperatureinduced Lifshitz transition provides a natural explanation on the origin of the transport property anomalies in ZrTe_{5}. Because there is an energy gap between the LB band and the UB band, and both bands shift with temperature (Fig. 2), it is clear that at high temperature, when the Fermi surface is a holelike pocket, it is a ptype semimetal. With decreasing temperature, when the holelike valence band sinks down to below the Fermi level and the Fermi level lies in the gapped region, ZrTe_{5} enters into a semiconducting state. At ∼135 K, the Fermi level lies close to the centre of the energy gap. With further decreasing of temperature, the UB conduction band moves downwards to touch the Fermi level. The Fermi surface becomes an electronlike pocket and ZrTe_{5} changes into an ntype semimetal at low temperature. Therefore, ZrTe_{5} undergoes a transition from a ptype semimetal at high temperature, to a semiconductor in a narrow temperature region around 135 K, to an ntype semimetal at low temperature. The temperature evolution of the spectral weight at the Fermi level (Fig. 3h) is consistent with this picture. We note that around 135 K the transport properties of ZrTe_{5} are mainly dictated by the bands near Γ point; the other β band does not cross the Fermi level until very low temperature that will add more electrons into ZrTe_{5} and further reduce its resistivity (Supplementary Figs 8 and 9). This provides a natural explanation on the resistivity maximum at ∼135 K in the transport measurement. It also accounts for the sign reversal of the Hall coefficient and thermopower^{4,6} because it corresponds to charge carrier change from ptype at high temperature to ntype at low temperature across ∼135 K.
Our present results pose a new issue on the origin of the chemical potential variation with temperature in ZrTe_{5}, that is, how temperature can induce a marked chemical potential shift in ZrTe_{5} without obvious charge carrier doping. In terms of usual understanding, our temperaturedependent results indicate that extra holes are present above ∼135 K, no carriers present in the semiconducting state around 135 K and extra electrons appear below ∼135 K. Without external doping mechanism, these seem to violate the charge balance in the temperature variation process. We believe the measured temperaturedependent behaviours represent intrinsic properties of ZrTe_{5}, not artefact caused by extrinsic factors like trivial absorption/desorption process. First, the measurements were performed in ultrahigh vacuum and in different ARPES systems; the results are reproducible. Second, the results are consistent with other ARPES results on similar ZrTe_{5} sample with similar resistivity anomaly temperature^{6,10}. Third, our ARPES measurements identified a Lifshitz transition at ∼135 K that corresponds to the resistivity anomaly temperature; it is hard to believe this is coincidental. Fourth, most importantly, our ARPES results are consistent with the bulk Hall coefficient and thermopower measurements that indicate a charge carrier change from holelike at high temperature to electronlike at low temperature across ∼135 K (refs 4, 5, 6). Such an unusual temperaturedependent chemical potential shift was considered to be a characteristic of an intrinsic semiconductor^{6}. It may also be related to charge carrier localization/delocalization on changing temperature. It is well known that the chemical potential can exhibit a significant shift with temperature in a degenerate semiconductor^{48}. It is possible that the ZrTe_{5} samples we measured contain defects or impurities; whether ZrTe_{5} really behaves like a degenerate semiconductor needs to be further explored. Considering similar temperature dependence of the bandgap (Fig. 2f) and the lattice parameter b (Fig. 3j), it is also interesting to investigate whether the variation of the interlayer interaction with temperature might give rise to such an unusual electronic state transition. While we do not have a clear answer on the origin yet, the marked charge carrier change with temperature may hide some deep physical mechanism that calls for further investigations.
Our detailed electronic structure measurements of ZrTe_{5} provide direct information to examine on the nature of its possible topological state, that is, whether it is a topological insulator^{37} or a quasitwodimensional^{41} or threedimensional Dirac semimetal^{38,39,40}. If ZrTe_{5} is a quasitwodimensional semimetal, one would observe a Dirac cone in the ac plane that we have measured. The absence of such a Dirac cone in our measurements clearly rules out such a scenario. For a similar reason, the gap opening between the LB valence band and the UB conduction band, especially its variation with temperature and its persistence down to the lowest temperature we measured (Fig. 2c,f) are not compatible with the threedimensional Dirac semimetal picture for ZrTe_{5}. Our electronic structure measurements are in good agreement with the transport measurements that show a resistivity anomaly and a reversal between electron and holelike charge carriers. One may argue whether the gap opening we observed is due to k_{z} effect because, in principle, the threedimensional Dirac cone can only be seen at particular k_{z} values. Our measurements using different photon energies indicate that k_{z} for the 6.994 eV laser is close to the basal k_{z}=0 plane (Supplementary Fig. 10). In particular, the gradual temperaturedependent change of the relative position between the UB and the LB bands near Γ point provides strong evidence on the gap opening, irrespective of k_{z} location, which is not consistent with the threedimensional Dirac cone picture for ZrTe_{5}. We note that the inconsistency on the nature of topological state in ZrTe_{5} may be due to sample difference. The ZrTe_{5} we measured here has a resistivity anomaly at ∼135 K that is consistent with most of the samples reported before^{2,3,4,6,7,8,9,10,41,42,44}, ^{45}. On the other hand, for the reports of threedimensional Dirac semimetal^{38,39,40}, the ZrTe_{5} samples were grown by a different method and exhibit a resistivity anomaly at a much lower temperature, ∼60 K. While our ARPES results are consistent with previous reports^{6,10} on the ZrTe_{5} samples with similar resistivity anomaly temperature ∼135 K, they are quite different from those on the ZrTe_{5} sample with a ∼60 K resistivity anomaly^{38}.
Band structure calculations predict that singlelayer ZrTe_{5} is a twodimensional topological insulator^{37}. Our ARPES results in Figs 1, 2, 3 are hard to provide a definitive answer on this issue because the ZrTe_{5} sample we measured is bulk instead of a singlelayer form. However, some additional quasionedimensional features we observed in some cleaved thin samples appear compatible with the edge states in ZrTe_{5}. For some cleaved thin ZrTe_{5} samples, there may appear some onedimensional line structures on the surface (Fig. 4a); the population of these structures can be further increased by deliberately cycling the sample temperature up and down many times. In these samples, we can observe additional bands growing on top of the original bulk bands (Fig. 4e). These extra bands form quasionedimensional intensity streaks running along the k_{y} direction, which is perpendicular to the onedimensional ZrTe_{6} chain direction that runs along a axis (Fig. 4b,c). When we rotated the sample, the quasionedimensional features also rotated simultaneously, indicating it is associated with the intrinsic property of ZrTe_{5} rather than an artefact or a photoemission matrix element effect (Supplementary Fig. 11). To firmly establish the validation of the quasionedimensional feature and its possible origin, we have carried out massive experiments with a plenty of samples. We found that the signal intensity of these extra bands varies among samples but its observation is quite common in samples with onedimensional thread structures on surface. The quasionedimensional feature appears only when the sample surfaces are cracked (by cycling of cooling and warming) with a bunch of edges; it is invisible in ZrTe_{5} with a smooth mirrorlike surface (Fig. 1). They are not present in the band structure calculations of the bulk ZrTe_{5} (Supplementary Fig. 4) either. These results indicate that the extra bands are closely associated with the onedimensional edges of the line structures on the ZrTe_{5} surface. There are some qualitative agreements between our measurements and the calculations. First, the extra holelike bands along Γ–X direction (Fig. 4e) are quite similar to those shown by the red line in Fig. 3d in ref. 37, which come from the edge of monolayer ZrTe_{5} with prismatic chain termination. Second, the measured bands have comparable Fermi momenta k_{F}’s and Fermi velocity with those in the calculations. Third, the edge state bands merge into the bulk bands at ∼150 meV binding energy in both our measurements and the calculations. These results lend more support on the edge states of our observation although further effort is needed to have a more quantitative comparison when the structure of the edges in the cracked ZrTe_{5} samples is known. Our observations are also consistent with the recent scanning tunnelling microscope experiments on ZrTe_{5} that reported observation of edge states on ZrTe_{5} surface^{49,50}. These results indicate that the extra quasionedimensional bands are consistent with the edge state of singlelayer ZrTe_{5} (ref. 37). They therefore suggest that ZrTe_{5} is a weak topological insulator that can be viewed as a stack of twodimensional topological insulator (or quantum spin Hall insulator) with topological edge mode.
We finally examine on possible temperatureinduced topological phase transition that is expected in ZrTe_{5} (ref. 37). Band structure calculations^{37} indicate that the topological property of ZrTe_{5} is sensitive to the interlayer coupling between the adjacent ZrTe_{5} layers and bulk ZrTe_{5} is sitting very close to the border between the weak and strong topological insulators. When the interlayer coupling is weak, bulk ZrTe_{5} acts as a threedimensional weak topological insulator. When the interlayer coupling gets strong, bulk ZrTe_{5} can be transformed into a threedimensional strong topological insulator like typical Bi_{2}Se_{3} and Bi_{2}Te_{3} threedimensional topological insulators^{51,52,53}. In this case, topological surface state is expected to appear, as shown in Supplementary Fig. 4c,e. With decreasing temperature, the lattice constant b decreases (Fig. 3j), the gap between the LB band and the UB band decreases (Fig. 2f); these results are consistent with the enhancement of the interlayer coupling as expected^{37}.
The topological transition from a weak to a strong threedimensional insulators asks that the LB and the UB bands at Γ point move close to each other with decreasing temperature, touch and merge together and then open a new gap after the band inversion. Our ARPES results (Fig. 2) indeed show a trend of gap closing with decreasing temperature, but we believe the gap persists over the entire temperature range that we have measured. One might argue that below 65 K, the filling up of the spectral weight at the valley bottom could be due to appearance of a new surface state that emerges in the new gapped region after the original gap is closed and the band inversion is realized. This possibility cannot be fully ruled out. To check on this possibility, we carefully searched for the possible signature of the topological surface state that would be expected inside the gap region near Γ point at ∼2 K. As seen from Supplementary Fig. 9b,e, no signature of the extra surface state can be resolved. Therefore, our results suggest that till the lowest temperature we measured (∼2 K), the gap between the LB band and the UB band near Γ remains open, and no band inversion has been realized in the measured temperature range. The observation of possible edge states in ZrTe_{5} at 15 K also indicates that ZrTe_{5} is a weak topological insulator (Fig. 4). The lattice shrinkage along b axis with temperature (Fig. 3j) by 0.3% is not enough for driving the topological phase transition to occur^{37}. Our present study indicates a clear trend of such a transition; further enhancement of the interlayer coupling is needed to materialize such a topological phase transition.
In summary, we have carried out comprehensive highresolution ARPES measurements on ZrTe_{5}. We have uncovered direct electronic evidence of a temperatureinduced Lifshitz transition in ZrTe_{5}. The sample undergoes a ptype semimetal to a semiconductor, to an ntypesemimetal transition with decreasing temperature. This evolution provides a natural explanation on the longstanding issue of the origin of the resistivity anomaly in ZrTe_{5}. It also indicates that ZrTe_{5} with a resistive anomaly at ∼135 K is not a threedimensional Dirac semimetal. We observed quasionedimensional electronic features that may be associated with the edge states of ZrTe_{5}. Such an observation, together with the persistence of bandgap opening, absence of Dirac surface states and no topological phase transition over the entire temperature range we measured, indicates that ZrTe_{5} is a weak topological insulator. With decreasing temperature, there is a tendency of the transition from a weak topological insulator to a strong topological insulator. Further enhancement of the interlayer coupling, either by external high pressure or internal chemical pressure, may facilitate the realization of such a topological phase transition.
Methods
Sample preparation
Highquality singlecrystal samples of ZrTe_{5} were grown by the chemical vapour transport method with iodine as transport agent. The unique resistivity peak sits at a temperature of ∼135 K (Fig. 1d), in good agreement with the typical values reported in most of the previous literatures^{2,3,4,6,7,8,9,10,41,42,44,45}.
Highresolution ARPES measurements
Most of ARPES measurements were performed at our new laserbased system equipped with the 6.994 eV vacuumultraviolet laser and the timeofflight electron energy analyser (ARToF 10 K by Scienta Omicron). This latestgeneration ARPES system is capable of measuring photoelectrons covering twodimensional momentum space (k_{x}, k_{y}) simultaneously. Measurements were performed using both s and ppolarization geometries. For the photon energydependent measurements, our tunablelaser ARPES system equipped with a hemispherical analyser DA30L (ScientaOmicron) was used with the photon energy varying in the range of 5.9 and 7.09 eV. The overall energy resolution was set at 1–5 meV, and the angular resolution was ∼0.1°. All the samples were measured in ultrahigh vacuum with a base pressure better than 5 × 10^{−11} mbar. The samples for temperaturedependent experiments were cleaved in situ at either 35 or 255 K and measured at temperatures ranging from 35 to 255 K. Samples measured at 15 or 2 K were cleaved in situ at 15 and 2 K, respectively. To avoid the hydrogen contamination on the sample surface at low temperature, during the ARPES measurements, we deliberately stay away from 20–33 K range near the hydrogenboiling temperature.
Band structure calculations
The band structure calculations were performed with the projector augmented wave method^{54,55} implemented in Vienna ab initio simulation package^{56,57}. The cutoff energy for the plane wave expansion is set to 450 eV. The generalized gradient approximation of Perdew–Burke–Ernzerhof type^{58} is used to deal with the exchange and correlation potential. The kpoint sampling grid in the selfconsistent process is 13 × 13 × 7. Spin Orbital Coupling (SOC) is included as a second vibrational step using scalar relativistic eigenfunctions as the bases after the initial calculation is achieved in the selfconsistent iterations. Maximally localized Wannier functions for the p orbitals of Te atoms have been constructed by using the WANNIER90 code^{59,60,61}. A slab tightbinding model has been constructed to calculate the surface states by using the Wannier functions.
Data availability
The authors declare that all data supporting the findings of this study are available within the paper and its Supplementary Information files.
Additional information
How to cite this article: Zhang, Y. et al. Electronic evidence of temperatureinduced Lifshitz transition and topological nature in ZrTe_{5}. Nat. Commun. 8, 15512 doi: 10.1038/ncomms15512 (2017).
Publisher’s note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
References
 1.
Furuseth, S., Brattas, L. & Kjejshus, A. The crystal structure of HfTe_{5}. Acta Chem. Scand. 27, 2367 (1973).
 2.
Weiting, T. J. et al. Giant anomalies in the resistivities of quasionedimensional ZrTe_{5} and HfTe_{5}. Bull Am. Phys. Soc. 25, 340 (1980).
 3.
Okada, S. et al. Giant resistivity anomaly in ZrTe_{5}. J. Phys. Soc. Jpn 49, 839 (1980).
 4.
Jones, T. E. et al. Thermoelectric power of HfTe_{5} and ZrTe_{5}. Solid State Commun. 42, 793–798 (1982).
 5.
Izumi, M. et al. Hall effect and transverse magnetoresistance in a lowdimensional conductor HfTe_{5}. Solid State Commun. 42, 773–778 (1982).
 6.
McIlroy, D. N. et al. Observation of a semimetalsemiconductor phase transition in the intermetallic ZrTe_{5}. J. Phys.: Condens. Matter 16, 359–365 (2004).
 7.
DiSalvo, F. J. et al. Possible phase transition in the quasionedimensional materials ZrTe_{5} and HfTe_{5}. Phys. Rev. B 24, 2935 (1981).
 8.
Okada, S. et al. Negative evidences for charge/spin density wave in ZrTe_{5}. J. Phys. Soc. Jpn 51, 460 (1982).
 9.
Rubinstein, M. ZrTe_{5} and HfTe_{5}: possible polaronic conductors. Phys. Rev. B 60, 1627 (1999).
 10.
Manzoni, G. et al. Ultrafast optical control of the electronic properties of ZrTe_{5}. Phys. Rev. Lett. 115, 207402 (2015).
 11.
Hasan, M. Z. & Kane, C. L. Colloquium: topological insulators. Rev. Mod. Phys. 82, 3045 (2010).
 12.
Qi, X. L. & Zhang, S. C. Topological insulators and superconductors. Rev. Mod. Phys. 83, 1057 (2011).
 13.
Ando, Y. Topological insulator materials. J. Phys. Soc. Jpn 82, 102001 (2013).
 14.
Burkov, A. A., Hook, M. D. & Balents, L. Topological nodal semimetals. Phys. Rev. B 84, 235126 (2011).
 15.
Young, S. M. et al. Dirac semimetal in three dimensions. Phys. Rev. Lett. 108, 140405 (2012).
 16.
Wang, Z. et al. Dirac semimetal and topological phase transitions in A_{3}Bi (A=Na, K, Rb). Phys. Rev. B 85, 195320 (2012).
 17.
Wang, Z., Weng, H., Wu, Q., Dai, X. & Fang, Z. Threedimensional Dirac semimetal and quantum transport in Cd_{3}As_{2}. Phys. Rev. B 88, 125427 (2013).
 18.
Liu, Z. K. et al. Discovery of a threedimensional topological Dirac semimetal, Na_{3}Bi. Science 343, 864–867 (2014).
 19.
Neupane, M. et al. Observation of a threedimensional topological Dirac semimetal phase in highmobility Cd_{3}As_{2}. Nat. Commun. 5, 3786 (2014).
 20.
Liu, Z. K. et al. A stable threedimensional topological Dirac semimetal Cd_{3}As_{2}. Nat. Mater. 13, 677–681 (2014).
 21.
Borisenko, S. et al. Experimental realization of a threedimensional Dirac semimetal. Phys. Rev. Lett. 113, 027603 (2014).
 22.
Yi, H. et al. Evidence of topological surface state in threedimensional Dirac semimetal Cd_{3}As_{2}. Sci. Rep. 4, 6106 (2014).
 23.
Xu, S. Y. et al. Observation of Fermi arc surface states in a topological metal. Science 347, 294 (2015).
 24.
Wan, X. et al. Topological semimetal and Fermiarc surface states in the electronic structure of pyrochlore iridates. Phys. Rev. B 83, 205101 (2011).
 25.
Burkov, A. A. & Balents, L. Weyl semimetal in a topological insulator multilayer. Phys. Rev. Lett. 107, 127205 (2011).
 26.
Huang, S. et al. A Weyl Fermion semimetal with surface Fermi arcs in the transition metal monopnictide TaAs class. Nat. Commun. 6, 7373 (2015).
 27.
Weng, H., Fang, C., Fang, Z., Bernevig, B. A. & Dai, X. Weyl semimetal phase in noncentrosymmetric transitionmetal monophosphides. Phys. Rev. X 5, 011029 (2015).
 28.
Xu, S. et al. Discovery of a Weyl fermion semimetal and topological Fermi arcs. Science 349, 613–617 (2015).
 29.
Lv, B. Q. et al. Experimental discovery of Weyl semimetal TaAs. Phys. Rev. X 5, 031013 (2015).
 30.
Yang, L. X. et al. Weyl semimetal phase in the noncentrosymmetric compound TaAs. Nat. Phys. 11, 728–732 (2015).
 31.
Lv, B. Q. et al. Observation of Weyl nodes in TaAs. Nat. Phys. 11, 724–728 (2015).
 32.
Xu, S. et al. Discovery of a Weyl Fermion state with Fermi arcs in niobium arsenide. Nat. Phys. 11, 748–754 (2015).
 33.
Xu, S.Y. et al. Experimental discovery of a topological Weyl semimetal state in TaP. Sci. Adv. 1, e1501092 (2015).
 34.
Bernevig, B. A., Hughes, T. L. & Zhang, S. C. Quantum spin Hall effect and topological phase transition in HgTe quantum wells. Science 314, 1757 (2006).
 35.
Koenig, M. et al. Quantum spin Hall insulator state in HgTe quantum wells. Science 318, 766 (2007).
 36.
Pauly, C. et al. Subnanometrewide electron channels protected by topology. Nat. Phys. 11, 338–343 (2015).
 37.
Weng, H. M., Dai, X. & Fang, Z. Transitionmetal pentatelluride ZrTe_{5} and HfTe_{5}: a paradigm for largegap quantum spin Hall insulators. Phys. Rev. X 4, 011002 (2014).
 38.
Li, Q. et al. Chiral magnetic effect in ZrTe_{5}. Nat. Phys. 12, 550–554 (2016).
 39.
Chen, R. Y. et al. Optical spectroscopy study of three dimensional Dirac semimetal ZrTe_{5}. Phys. Rev. B 92, 075107 (2015).
 40.
Chen, R. Y. et al. Magnetoinfrared spectroscopy of Landau levels and Zeeman splitting of threedimensional massless Dirac Fermions in ZrTe_{5}. Phys. Rev. Lett. 115, 176404 (2015).
 41.
Yuan, X. et al. Observation of quasitwodimensional Dirac fermions in ZrTe_{5}. NPG Asia Mater. 8, e325 (2016).
 42.
Zhou, Y. H. et al. Pressureinduced semimetal to superconductor transition in a threedimensional topological material ZrTe_{5}. Proc. Natl Acad. Sci. USA 113, 2904–2909 (2016).
 43.
Damascelli, A., Hussain, Z. & Shen, Z. X. Angleresolved photoemission studies of the cuprate superconductors. Rev. Mod. Phys. 75, 473 (2003).
 44.
Kamm, G. N. et al. Fermi surface, effective masses, and Dingle temperatures of ZrTe_{5} as derived from the Shubnikovde Haas effect. Phys. Rev. B 31, 7617 (1985).
 45.
Mitsuru, I. et al. Shubnikovde Haas oscillations and Fermi surfaces in transitionmetal pentatellurides ZrTe_{5}, and HfTe_{5}. J. Phys. C: Solid State Phys. 20, 3691–3705 (1987).
 46.
Whangbo, M. H. et al. Electronic structure of ZrTe_{5}. Phys. Rev. B 26, 687 (1982).
 47.
Wu, Y. et al. Temperatureinduced Lifshitz transition in WTe_{2}. Phys. Rev. Lett. 115, 166602 (2015).
 48.
Colinge, J. P. & Colinge, C. A. in Physics of Semiconductor Devices Kluwer (2002).
 49.
Li, X.B. et al. Experimental observation of topological edge states at the surface step edge of the topological insulator ZrTe_{5}. Phys. Rev. Lett. 116, 176803 (2016).
 50.
Wu, R. et al. Evidence for topological edge state in a large energy gap near the step edges on the surface of ZrTe_{5}. Phys. Rev. X 6, 021017 (2016).
 51.
Zhang, H. J. et al. Topological insulators in Bi_{2}Se_{3}, Bi_{2}Te_{3} and Sb_{2}Te_{3} with a single Dirac cone on the surface. Nat. Phys. 5, 438–442 (2009).
 52.
Xia, Y. et al. Observation of a largegap topological insulator class with a single Dirac cone on the surface. Nat. Phys. 5, 398–402 (2009).
 53.
Chen, Y. L. et al. Experimental realization of a threedimensional topological insulator, Bi_{2}Te_{3}. Science 325, 178–181 (2009).
 54.
Blöchl, P. E. Projector augmentedwave method. Phys. Rev. B 50, 17953 (1994).
 55.
Kresse, G. et al. From ultrasoft pseudopotentials to the projector augmentedwave method. Phys. Rev. B 59, 1758 (1999).
 56.
Kresse, G. et al. Efficiency of abinitio total energy calculations for metals and semiconductors using a planewave basis set. Comput. Mater. Sci. 6, 15 (1996).
 57.
Kresse, G. et al. Efficient iterative schemes for ab initio totalenergy calculations using a planewave basis set. Phys. Rev. B 54, 11169 (1996).
 58.
Perdew, J. et al. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865 (1996).
 59.
Marzari, N. et al. Maximally localized generalized Wannier functions for composite energy bands. Phys. Rev. B 56, 12847 (1997).
 60.
Souza, I. et al. Maximally localized Wannier functions for entangled energy bands. Phys. Rev. B 65, 035109 (2001).
 61.
Mostofi, A. et al. wannier90: a tool for obtaining maximallylocalised Wannier functions. Comp. Phys. Commun. 178, 685 (2008).
 62.
Fjellvalg, H. et al. Structure properties of ZrTe_{5} and HfTe_{5} as seen by powder diffraction. Solid State Commun. 60, 91–93 (1986).
Acknowledgements
This work is supported by the National Science Foundation of China (11574367), the 973 project of the Ministry of Science and Technology of China (2013CB921700, 2013CB921904 and 2015CB921300) and the Strategic Priority Research Program (B) of the Chinese Academy of Sciences (Grant No. XDB07020300).
Author information
Author notes
 Yan Zhang
 , Chenlu Wang
 & Li Yu
These authors contributed equally to this work
Affiliations
Beijing National Laboratory for Condensed Matter Physics, Institute of Physics, Chinese Academy of Sciences, Beijing 100190, China
 Yan Zhang
 , Chenlu Wang
 , Li Yu
 , Guodong Liu
 , Aiji Liang
 , Jianwei Huang
 , Simin Nie
 , Xuan Sun
 , Yuxiao Zhang
 , Bing Shen
 , Jing Liu
 , Hongming Weng
 , Lingxiao Zhao
 , Genfu Chen
 , Cheng Hu
 , Ying Ding
 , Wenjuan Zhao
 , Qiang Gao
 , Cong Li
 , Shaolong He
 , Lin Zhao
 , Xi Dai
 , Zhong Fang
 & X. J. Zhou
University of Chinese Academy of Sciences, Beijing 100049, China
 Yan Zhang
 , Chenlu Wang
 , Jianwei Huang
 , Xuan Sun
 , Bing Shen
 , Jing Liu
 , Cheng Hu
 , Ying Ding
 , Wenjuan Zhao
 , Qiang Gao
 , Cong Li
 & X. J. Zhou
Collaborative Innovation Center of Quantum Matter, Beijing 100871, China
 Hongming Weng
 , Genfu Chen
 , Xi Dai
 , Zhong Fang
 & X. J. Zhou
Military Transportation University, Tianjin 300161, China
 Xiaowen Jia
Technical Institute of Physics and Chemistry, Chinese Academy of Sciences, Beijing 100190, China
 Fengfeng Zhang
 , Shenjin Zhang
 , Feng Yang
 , Zhimin Wang
 , Qinjun Peng
 , Zuyan Xu
 & Chuangtian Chen
Authors
Search for Yan Zhang in:
Search for Chenlu Wang in:
Search for Li Yu in:
Search for Guodong Liu in:
Search for Aiji Liang in:
Search for Jianwei Huang in:
Search for Simin Nie in:
Search for Xuan Sun in:
Search for Yuxiao Zhang in:
Search for Bing Shen in:
Search for Jing Liu in:
Search for Hongming Weng in:
Search for Lingxiao Zhao in:
Search for Genfu Chen in:
Search for Xiaowen Jia in:
Search for Cheng Hu in:
Search for Ying Ding in:
Search for Wenjuan Zhao in:
Search for Qiang Gao in:
Search for Cong Li in:
Search for Shaolong He in:
Search for Lin Zhao in:
Search for Fengfeng Zhang in:
Search for Shenjin Zhang in:
Search for Feng Yang in:
Search for Zhimin Wang in:
Search for Qinjun Peng in:
Search for Xi Dai in:
Search for Zhong Fang in:
Search for Zuyan Xu in:
Search for Chuangtian Chen in:
Search for X. J. Zhou in:
Contributions
Y.Z., C.L.W. and L.Y. contribute equally to this work. X.J.Z., G.D.L., Y.Z., C.L.W., L.Y., A.J.L. and J.W.H. proposed and designed the research; L.X.Z. and G.F.C. contributed in sample growth; S.M.N., H.W.M., X.D. and Z.F. contributed to the band structure calculations; Y.Z., C.L.W., L.Y., G.D.L., A.J.L., J.W.H., X.S., Y.X.Z., B.S., J.L., X.W.J., C.H., Y.D., W.J.Z., Q.G., C.L., S.L.H., L.Z., F.F.Z., S.J.Z., F.Y., Z.M.W., Q.J.P., Z.Y.X., C.T.C. and X.J.Z. contributed to the development and maintenance of the LaserARTOF system and related software development; Y.Z., C.L.W., J.W.H. and A.J.L. carried out the ARPES experiment; Y.Z., C.L.W., L.Y., G.D.L., A.J.L. and X.J.Z. analysed the data; X.J.Z., G.D.L. and Y.Z. wrote the paper with C.L.W., L.Y., A.J.L., S.M.N. and H.M.W. All authors participated in discussion and comment on the paper.
Competing interests
The authors declare no competing financial interests.
Corresponding authors
Correspondence to Guodong Liu or X. J. Zhou.
Supplementary information
PDF files
 1.
Supplementary Information
Supplementary Figures, Supplementary Notes, Supplementary References.
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Further reading

Quantum Oscillations from Nontrivial States in QuasiTwoDimensional Dirac Semimetal ZrTe5 Nanowires
Scientific Reports (2019)

Pressureinduced Lifshitz transition in the type II Dirac semimetal PtTe2
Science China Physics, Mechanics & Astronomy (2019)

Turning ZrTe5 into a semiconductor through atom intercalation
Science China Physics, Mechanics & Astronomy (2019)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.